 
data_musc_new_295k
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
;
 ?
;
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'H1.83 Al2.49 F0 Fe0.32 K Na0 O12 Si3.26'
_chemical_formula_weight          397.71
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'K'  'K'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O'  'O'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'F'  'F'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            ?
_symmetry_space_group_name_H-M    ?
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, y, -z+1/2'
 'x+1/2, y+1/2, z'
 '-x+1/2, y+1/2, -z+1/2'
 '-x, -y, -z'
 'x, -y, z-1/2'
 '-x+1/2, -y+1/2, -z'
 'x+1/2, -y+1/2, z-1/2'
 
_cell_length_a                    5.2093(2)
_cell_length_b                    9.0391(4)
_cell_length_c                    20.0343(7)
_cell_angle_alpha                 90.00
_cell_angle_beta                  95.782(2)
_cell_angle_gamma                 90.00
_cell_volume                      938.56(6)
_cell_formula_units_Z             4
_cell_measurement_temperature     295(2)
_cell_measurement_reflns_used     ?
_cell_measurement_theta_min       ?
_cell_measurement_theta_max       ?
 
_exptl_crystal_description        ?
_exptl_crystal_colour             ?
_exptl_crystal_size_max           ?
_exptl_crystal_size_mid           ?
_exptl_crystal_size_min           ?
_exptl_crystal_density_meas       ?
_exptl_crystal_density_diffrn     ?
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              ?
_exptl_absorpt_coefficient_mu     0.000
_exptl_absorpt_correction_type    ?
_exptl_absorpt_correction_T_min   ?
_exptl_absorpt_correction_T_max   ?
_exptl_absorpt_process_details    ?
 
_exptl_special_details
;
 ?
;
 
_diffrn_ambient_temperature       295(2)
_diffrn_radiation_wavelength      0.9462
_diffrn_radiation_type            ?
_diffrn_radiation_source          'CW neutron D19-ILL'
_diffrn_radiation_monochromator   ?
_diffrn_measurement_device_type   ?
_diffrn_measurement_method        ?
_diffrn_detector_area_resol_mean  ?
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             9727
_diffrn_reflns_av_R_equivalents   0.1090
_diffrn_reflns_av_sigmaI/netI     0.0564
_diffrn_reflns_limit_h_min        -5
_diffrn_reflns_limit_h_max        7
_diffrn_reflns_limit_k_min        -11
_diffrn_reflns_limit_k_max        13
_diffrn_reflns_limit_l_min        -29
_diffrn_reflns_limit_l_max        29
_diffrn_reflns_theta_min          6.01
_diffrn_reflns_theta_max          44.98
_reflns_number_total              1631
_reflns_number_gt                 1431
_reflns_threshold_expression      >2sigma(I)
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         ?
_computing_structure_solution     ?
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.0100P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_atom_sites_solution_hydrogens    geom
_refine_ls_hydrogen_treatment     mixed
_refine_ls_extinction_method      SHELXL
_refine_ls_extinction_coef        0.0041(8)
_refine_ls_extinction_expression
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
_refine_ls_number_reflns          1631
_refine_ls_number_parameters      109
_refine_ls_number_restraints      0
_refine_ls_R_factor_all           0.0806
_refine_ls_R_factor_gt            0.0718
_refine_ls_wR_factor_ref          0.1382
_refine_ls_wR_factor_gt           0.1370
_refine_ls_goodness_of_fit_ref    2.694
_refine_ls_restrained_S_all       2.694
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
K K 0.0000 0.0977(5) 0.2500 0.0310(11) Uani 0.998(19) 2 d SP . .
Al Al 0.2501(3) 0.08334(19) -0.00006(8) 0.0144(5) Uani 0.876(8) 1 d P . .
Fe Fe 0.2501(3) 0.08334(19) -0.00006(8) 0.0144(5) Uani 0.124(8) 1 d P . .
Si2 Si 0.4518(3) 0.2582(2) 0.13552(9) 0.0156(5) Uani 0.88(6) 1 d P . .
Al2 Al 0.4518(3) 0.2582(2) 0.13552(9) 0.0156(5) Uani 0.12(6) 1 d P . .
O1 O 0.4256(3) 0.09302(17) 0.16854(7) 0.0231(3) Uani 1 1 d . . .
O3 O 0.2449(2) 0.36594(18) 0.16870(7) 0.0230(3) Uani 1 1 d . . .
O5 O 0.3891(2) 0.25131(16) 0.05363(7) 0.0183(3) Uani 1 1 d . . .
Si1 Si -0.5355(3) -0.0707(2) 0.13558(9) 0.0145(5) Uani 0.76(6) 1 d P . .
Al1 Al -0.5355(3) -0.0707(2) 0.13558(9) 0.0145(5) Uani 0.24(6) 1 d P . .
O2 O -0.7550(2) -0.18407(19) 0.15885(8) 0.0249(3) Uani 1 1 d . . .
O4 O -0.5406(2) -0.05835(16) 0.05360(7) 0.0185(3) Uani 1 1 d . . .
O6 O 0.0441(2) 0.06391(17) 0.44898(7) 0.0211(3) Uani 1 1 d . . .
H H 0.1311(7) 0.1527(4) 0.4420(2) 0.0506(15) Uani 0.914(16) 1 d P . .
M1 Fe 0.2500 0.2500 0.5000 0.058(13) Uani 0.067(9) 2 d SP . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
K O1 2.8827(14) 2 ?
K O1 2.8827(14) . ?
K O3 2.893(3) 3_445 ?
K O3 2.893(3) 4_545 ?
K O2 2.916(3) 4_455 ?
K O2 2.916(3) 3 ?
K O3 3.253(4) 2 ?
K O3 3.253(4) . ?
K O1 3.2611(14) 1_455 ?
K O1 3.2611(14) 2_655 ?
K O2 3.453(4) 1_655 ?
K O2 3.453(4) 2_455 ?
Al O6 1.935(2) 2 ?
Al O6 1.935(2) 6 ?
Al O4 1.936(2) 1_655 ?
Al O5 1.938(2) 7 ?
Al O4 1.954(2) 5 ?
Al O5 1.957(2) . ?
Al Al 3.008(3) 5_655 ?
Al Fe 3.008(3) 5_655 ?
Al M1 3.0082(15) 2_655 ?
Al M1 3.0097(15) 2 ?
Al Fe 3.011(3) 5 ?
Al Al 3.011(3) 5 ?
Si2 O2 1.637(2) 3_655 ?
Si2 O5 1.641(2) . ?
Si2 O3 1.642(2) . ?
Si2 O1 1.644(2) . ?
Si2 Al1 2.973(3) 1_655 ?
Si2 Si1 2.973(3) 1_655 ?
Si2 Al1 2.973(2) 3 ?
Si2 Si1 2.973(2) 3 ?
Si2 Al1 3.086(2) 3_655 ?
Si2 Si1 3.086(2) 3_655 ?
Si2 Al 3.154(2) 7 ?
Si2 Fe 3.154(2) 7 ?
O1 Al1 1.641(2) 1_655 ?
O1 Si1 1.641(2) 1_655 ?
O1 O2 2.633(2) 3_655 ?
O1 O3 2.640(2) . ?
O1 O3 2.642(2) 3_545 ?
O1 O2 2.676(2) 1_655 ?
O1 O4 2.700(2) 1_655 ?
O1 O5 2.701(2) . ?
O1 O6 3.2310(19) 2 ?
O3 Al1 1.646(2) 3 ?
O3 Si1 1.646(2) 3 ?
O3 O2 2.6309(18) 3 ?
O3 O1 2.642(2) 3_455 ?
O3 O2 2.6709(18) 3_655 ?
O3 O5 2.7020(19) . ?
O3 O4 2.7033(19) 3 ?
O3 K 2.893(3) 3 ?
O3 O6 3.239(2) 4 ?
O5 Fe 1.938(2) 7 ?
O5 Al 1.938(2) 7 ?
O5 M1 2.2575(12) 2_655 ?
O5 O5 2.468(3) 7 ?
O5 O2 2.7268(18) 3_655 ?
O5 O6 2.8181(19) 2 ?
Si1 O2 1.638(2) . ?
Si1 O1 1.641(2) 1_455 ?
Si1 O4 1.644(2) . ?
Si1 O3 1.646(2) 3_445 ?
Si1 Al2 2.973(3) 1_455 ?
Si1 Si2 2.973(3) 1_455 ?
Si1 Al2 2.973(2) 3_445 ?
Si1 Si2 2.973(2) 3_445 ?
Si1 Al2 3.086(2) 3_345 ?
Si1 Si2 3.086(2) 3_345 ?
Si1 Fe 3.156(2) 1_455 ?
Si1 Al 3.156(2) 1_455 ?
O2 Al2 1.637(2) 3_345 ?
O2 Si2 1.637(2) 3_345 ?
O2 O3 2.6309(18) 3_445 ?
O2 O1 2.633(2) 3_345 ?
O2 O3 2.6709(18) 3_345 ?
O2 O1 2.676(2) 1_455 ?
O2 O5 2.7268(18) 3_345 ?
O2 O4 2.731(2) . ?
O2 K 2.916(3) 3_445 ?
O2 M1 3.2404(16) 4_445 ?
O4 Fe 1.936(2) 1_455 ?
O4 Al 1.936(2) 1_455 ?
O4 Fe 1.954(2) 5 ?
O4 Al 1.954(2) 5 ?
O4 M1 2.2600(14) 4_445 ?
O4 O4 2.467(3) 5_455 ?
O4 O1 2.700(2) 1_455 ?
O4 O3 2.7033(19) 3_445 ?
O4 O6 2.8179(19) 2 ?
O6 Fe 1.935(2) 2 ?
O6 Al 1.935(2) 2 ?
O6 Fe 1.935(2) 6_556 ?
O6 Al 1.935(2) 6_556 ?
O6 M1 2.1917(15) . ?
O6 O6 2.432(3) 5_556 ?
O6 O4 2.8179(19) 2 ?
O6 O5 2.8181(19) 2 ?
O6 O4 2.8419(19) 2_455 ?
O6 O5 2.848(2) 4_545 ?
O6 O4 2.8567(18) 6_656 ?
O6 O5 2.860(2) 8_456 ?
M1 O6 2.1917(15) 7_556 ?
M1 O5 2.2575(12) 8_456 ?
M1 O5 2.2575(12) 2_655 ?
M1 O4 2.2600(14) 6_656 ?
M1 O4 2.2600(14) 4_455 ?
M1 Al 3.0082(15) 8_456 ?
M1 Al 3.0082(15) 2_655 ?
M1 Fe 3.0082(15) 8_456 ?
M1 Fe 3.0082(15) 2_655 ?
M1 Al 3.0097(15) 2 ?
M1 Al 3.0097(15) 8_556 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O1 K O1 178.32(18) 2 . ?
O1 K O3 88.41(7) 2 3_445 ?
O1 K O3 90.37(7) . 3_445 ?
O1 K O3 90.37(7) 2 4_545 ?
O1 K O3 88.41(7) . 4_545 ?
O3 K O3 87.22(13) 3_445 4_545 ?
O1 K O2 89.03(7) 2 4_455 ?
O1 K O2 92.10(7) . 4_455 ?
O3 K O2 175.44(11) 3_445 4_455 ?
O3 K O2 89.02(4) 4_545 4_455 ?
O1 K O2 92.10(7) 2 3 ?
O1 K O2 89.03(7) . 3 ?
O3 K O2 89.02(4) 3_445 3 ?
O3 K O2 175.44(11) 4_545 3 ?
O2 K O2 94.85(14) 4_455 3 ?
O1 K O3 50.54(5) 2 2 ?
O1 K O3 131.10(14) . 2 ?
O3 K O3 129.838(15) 3_445 2 ?
O3 K O3 116.04(5) 4_545 2 ?
O2 K O3 50.13(6) 4_455 2 ?
O2 K O3 68.43(9) 3 2 ?
O1 K O3 131.10(14) 2 . ?
O1 K O3 50.54(5) . . ?
O3 K O3 116.04(5) 3_445 . ?
O3 K O3 129.838(15) 4_545 . ?
O2 K O3 68.43(9) 4_455 . ?
O2 K O3 50.13(6) 3 . ?
O3 K O3 83.60(11) 2 . ?
O1 K O1 64.14(5) 2 1_455 ?
O1 K O1 115.83(5) . 1_455 ?
O3 K O1 50.41(4) 3_445 1_455 ?
O3 K O1 128.21(13) 4_545 1_455 ?
O2 K O1 131.25(12) 4_455 1_455 ?
O2 K O1 50.08(4) 3 1_455 ?
O3 K O1 82.75(6) 2 1_455 ?
O3 K O1 98.37(7) . 1_455 ?
O1 K O1 115.83(5) 2 2_655 ?
O1 K O1 64.14(5) . 2_655 ?
O3 K O1 128.21(13) 3_445 2_655 ?
O3 K O1 50.41(4) 4_545 2_655 ?
O2 K O1 50.08(4) 4_455 2_655 ?
O2 K O1 131.25(12) 3 2_655 ?
O3 K O1 98.37(7) 2 2_655 ?
O3 K O1 82.75(6) . 2_655 ?
O1 K O1 178.51(16) 1_455 2_655 ?
O1 K O2 129.42(13) 2 1_655 ?
O1 K O2 48.95(5) . 1_655 ?
O3 K O2 48.81(6) 3_445 1_655 ?
O3 K O2 65.82(8) 4_545 1_655 ?
O2 K O2 131.37(2) 4_455 1_655 ?
O2 K O2 109.70(5) 3 1_655 ?
O3 K O2 177.99(5) 2 1_655 ?
O3 K O2 95.77(4) . 1_655 ?
O1 K O2 95.46(7) 1_455 1_655 ?
O1 K O2 83.43(6) 2_655 1_655 ?
O1 K O2 48.95(5) 2 2_455 ?
O1 K O2 129.42(13) . 2_455 ?
O3 K O2 65.82(8) 3_445 2_455 ?
O3 K O2 48.81(6) 4_545 2_455 ?
O2 K O2 109.70(5) 4_455 2_455 ?
O2 K O2 131.37(2) 3 2_455 ?
O3 K O2 95.77(4) 2 2_455 ?
O3 K O2 177.99(5) . 2_455 ?
O1 K O2 83.43(6) 1_455 2_455 ?
O1 K O2 95.46(7) 2_655 2_455 ?
O2 K O2 84.93(11) 1_655 2_455 ?
O6 Al O6 77.86(9) 2 6 ?
O6 Al O4 94.47(9) 2 1_655 ?
O6 Al O4 95.12(9) 6 1_655 ?
O6 Al O5 95.20(9) 2 7 ?
O6 Al O5 94.68(9) 6 7 ?
O4 Al O5 167.48(11) 1_655 7 ?
O6 Al O4 168.06(12) 2 5 ?
O6 Al O4 92.86(9) 6 5 ?
O4 Al O4 78.72(9) 1_655 5 ?
O5 Al O4 93.01(9) 7 5 ?
O6 Al O5 92.79(9) 2 . ?
O6 Al O5 168.07(10) 6 . ?
O4 Al O5 92.96(9) 1_655 . ?
O5 Al O5 78.64(8) 7 . ?
O4 Al O5 97.32(8) 5 . ?
O6 Al Al 133.30(11) 2 5_655 ?
O6 Al Al 95.15(9) 6 5_655 ?
O4 Al Al 39.58(5) 1_655 5_655 ?
O5 Al Al 131.49(11) 7 5_655 ?
O4 Al Al 39.14(5) 5 5_655 ?
O5 Al Al 96.66(8) . 5_655 ?
O6 Al Fe 133.30(11) 2 5_655 ?
O6 Al Fe 95.15(9) 6 5_655 ?
O4 Al Fe 39.58(5) 1_655 5_655 ?
O5 Al Fe 131.49(11) 7 5_655 ?
O4 Al Fe 39.14(5) 5 5_655 ?
O5 Al Fe 96.66(8) . 5_655 ?
Al Al Fe 0.00(9) 5_655 5_655 ?
O6 Al M1 141.00(9) 2 2_655 ?
O6 Al M1 141.14(9) 6 2_655 ?
O4 Al M1 83.81(6) 1_655 2_655 ?
O5 Al M1 83.67(6) 7 2_655 ?
O4 Al M1 48.70(5) 5 2_655 ?
O5 Al M1 48.62(5) . 2_655 ?
Al Al M1 60.12(5) 5_655 2_655 ?
Fe Al M1 60.12(5) 5_655 2_655 ?
O6 Al M1 46.63(5) 2 2 ?
O6 Al M1 84.86(7) 6 2 ?
O4 Al M1 140.34(9) 1_655 2 ?
O5 Al M1 48.58(5) 7 2 ?
O4 Al M1 140.93(9) 5 2 ?
O5 Al M1 83.32(6) . 2 ?
Al Al M1 179.92(11) 5_655 2 ?
Fe Al M1 179.92(11) 5_655 2 ?
M1 Al M1 119.91(6) 2_655 2 ?
O6 Al Fe 38.93(6) 2 5 ?
O6 Al Fe 38.93(6) 6 5 ?
O4 Al Fe 96.17(9) 1_655 5 ?
O5 Al Fe 96.36(9) 7 5 ?
O4 Al Fe 131.37(11) 5 5 ?
O5 Al Fe 131.31(11) . 5 ?
Al Al Fe 119.90(11) 5_655 5 ?
Fe Al Fe 119.90(11) 5_655 5 ?
M1 Al Fe 179.93(11) 2_655 5 ?
M1 Al Fe 60.07(5) 2 5 ?
O6 Al Al 38.93(6) 2 5 ?
O6 Al Al 38.93(6) 6 5 ?
O4 Al Al 96.17(9) 1_655 5 ?
O5 Al Al 96.36(9) 7 5 ?
O4 Al Al 131.37(11) 5 5 ?
O5 Al Al 131.31(11) . 5 ?
Al Al Al 119.90(11) 5_655 5 ?
Fe Al Al 119.90(11) 5_655 5 ?
M1 Al Al 179.93(11) 2_655 5 ?
M1 Al Al 60.07(5) 2 5 ?
Fe Al Al 0.00(8) 5 5 ?
O2 Si2 O5 112.54(12) 3_655 . ?
O2 Si2 O3 109.07(14) 3_655 . ?
O5 Si2 O3 110.75(11) . . ?
O2 Si2 O1 106.72(12) 3_655 . ?
O5 Si2 O1 110.59(13) . . ?
O3 Si2 O1 106.94(12) . . ?
O2 Si2 Al1 107.38(10) 3_655 1_655 ?
O5 Si2 Al1 87.99(9) . 1_655 ?
O3 Si2 Al1 127.48(11) . 1_655 ?
O1 Si2 Al1 25.15(7) . 1_655 ?
O2 Si2 Si1 107.38(10) 3_655 1_655 ?
O5 Si2 Si1 87.99(9) . 1_655 ?
O3 Si2 Si1 127.48(11) . 1_655 ?
O1 Si2 Si1 25.15(7) . 1_655 ?
Al1 Si2 Si1 0.000(2) 1_655 1_655 ?
O2 Si2 Al1 127.31(11) 3_655 3 ?
O5 Si2 Al1 86.33(8) . 3 ?
O3 Si2 Al1 25.30(7) . 3 ?
O1 Si2 Al1 111.53(9) . 3 ?
Al1 Si2 Al1 122.63(7) 1_655 3 ?
Si1 Si2 Al1 122.63(7) 1_655 3 ?
O2 Si2 Si1 127.31(11) 3_655 3 ?
O5 Si2 Si1 86.33(8) . 3 ?
O3 Si2 Si1 25.30(7) . 3 ?
O1 Si2 Si1 111.53(9) . 3 ?
Al1 Si2 Si1 122.63(7) 1_655 3 ?
Si1 Si2 Si1 122.63(7) 1_655 3 ?
Al1 Si2 Si1 0.00(7) 3 3 ?
O2 Si2 Al1 19.54(7) 3_655 3_655 ?
O5 Si2 Al1 95.99(9) . 3_655 ?
O3 Si2 Al1 107.79(10) . 3_655 ?
O1 Si2 Al1 124.19(10) . 3_655 ?
Al1 Si2 Al1 118.82(7) 1_655 3_655 ?
Si1 Si2 Al1 118.82(7) 1_655 3_655 ?
Al1 Si2 Al1 118.55(8) 3 3_655 ?
Si1 Si2 Al1 118.55(8) 3 3_655 ?
O2 Si2 Si1 19.54(7) 3_655 3_655 ?
O5 Si2 Si1 95.99(9) . 3_655 ?
O3 Si2 Si1 107.79(10) . 3_655 ?
O1 Si2 Si1 124.19(10) . 3_655 ?
Al1 Si2 Si1 118.82(7) 1_655 3_655 ?
Si1 Si2 Si1 118.82(7) 1_655 3_655 ?
Al1 Si2 Si1 118.55(8) 3 3_655 ?
Si1 Si2 Si1 118.55(8) 3 3_655 ?
Al1 Si2 Si1 0.00(9) 3_655 3_655 ?
O2 Si2 Al 108.75(10) 3_655 7 ?
O5 Si2 Al 30.86(7) . 7 ?
O3 Si2 Al 84.44(9) . 7 ?
O1 Si2 Al 136.44(11) . 7 ?
Al1 Si2 Al 117.38(7) 1_655 7 ?
Si1 Si2 Al 117.38(7) 1_655 7 ?
Al1 Si2 Al 63.46(6) 3 7 ?
Si1 Si2 Al 63.46(6) 3 7 ?
Al1 Si2 Al 89.21(6) 3_655 7 ?
Si1 Si2 Al 89.21(6) 3_655 7 ?
O2 Si2 Fe 108.75(10) 3_655 7 ?
O5 Si2 Fe 30.86(7) . 7 ?
O3 Si2 Fe 84.44(9) . 7 ?
O1 Si2 Fe 136.44(11) . 7 ?
Al1 Si2 Fe 117.38(7) 1_655 7 ?
Si1 Si2 Fe 117.38(7) 1_655 7 ?
Al1 Si2 Fe 63.46(6) 3 7 ?
Si1 Si2 Fe 63.46(6) 3 7 ?
Al1 Si2 Fe 89.21(6) 3_655 7 ?
Si1 Si2 Fe 89.21(6) 3_655 7 ?
Al Si2 Fe 0.00(8) 7 7 ?
Al1 O1 Si1 0.00(13) 1_655 1_655 ?
Al1 O1 Si2 129.65(13) 1_655 . ?
Si1 O1 Si2 129.65(13) 1_655 . ?
Al1 O1 O2 123.77(10) 1_655 3_655 ?
Si1 O1 O2 123.77(10) 1_655 3_655 ?
Si2 O1 O2 36.56(7) . 3_655 ?
Al1 O1 O3 154.32(11) 1_655 . ?
Si1 O1 O3 154.32(11) 1_655 . ?
Si2 O1 O3 36.50(7) . . ?
O2 O1 O3 60.86(6) 3_655 . ?
Al1 O1 O3 36.56(7) 1_655 3_545 ?
Si1 O1 O3 36.56(7) 1_655 3_545 ?
Si2 O1 O3 128.92(10) . 3_545 ?
O2 O1 O3 101.07(7) 3_655 3_545 ?
O3 O1 O3 161.87(9) . 3_545 ?
Al1 O1 O2 35.27(7) 1_655 1_655 ?
Si1 O1 O2 35.27(7) 1_655 1_655 ?
Si2 O1 O2 149.73(11) . 1_655 ?
O2 O1 O2 158.63(9) 3_655 1_655 ?
O3 O1 O2 138.76(7) . 1_655 ?
O3 O1 O2 59.30(5) 3_545 1_655 ?
Al1 O1 O4 34.76(8) 1_655 1_655 ?
Si1 O1 O4 34.76(8) 1_655 1_655 ?
Si2 O1 O4 95.84(9) . 1_655 ?
O2 O1 O4 103.24(7) 3_655 1_655 ?
O3 O1 O4 121.90(7) . 1_655 ?
O3 O1 O4 60.80(5) 3_545 1_655 ?
O2 O1 O4 61.07(5) 1_655 1_655 ?
Al1 O1 O5 97.79(10) 1_655 . ?
Si1 O1 O5 97.79(10) 1_655 . ?
Si2 O1 O5 34.67(8) . . ?
O2 O1 O5 61.48(5) 3_655 . ?
O3 O1 O5 60.76(5) . . ?
O3 O1 O5 113.76(7) 3_545 . ?
O2 O1 O5 116.11(7) 1_655 . ?
O4 O1 O5 63.03(5) 1_655 . ?
Al1 O1 K 111.97(12) 1_655 . ?
Si1 O1 K 111.97(12) 1_655 . ?
Si2 O1 K 108.31(12) . . ?
O2 O1 K 123.94(10) 3_655 . ?
O3 O1 K 72.00(10) . . ?
O3 O1 K 122.06(10) 3_545 . ?
O2 O1 K 76.70(10) 1_655 . ?
O4 O1 K 127.61(8) 1_655 . ?
O5 O1 K 118.86(8) . . ?
Al1 O1 O6 75.43(8) 1_655 2 ?
Si1 O1 O6 75.43(8) 1_655 2 ?
Si2 O1 O6 82.43(8) . 2 ?
O2 O1 O6 116.52(6) 3_655 2 ?
O3 O1 O6 80.39(6) . 2 ?
O3 O1 O6 111.60(6) 3_545 2 ?
O2 O1 O6 68.65(5) 1_655 2 ?
O4 O1 O6 56.41(5) 1_655 2 ?
O5 O1 O6 55.87(5) . 2 ?
K O1 O6 81.06(4) . 2 ?
Si2 O3 Al1 129.46(13) . 3 ?
Si2 O3 Si1 129.46(13) . 3 ?
Al1 O3 Si1 0.00(14) 3 3 ?
Si2 O3 O2 123.55(11) . 3 ?
Al1 O3 O2 36.65(8) 3 3 ?
Si1 O3 O2 36.65(8) 3 3 ?
Si2 O3 O1 36.55(8) . . ?
Al1 O3 O1 128.82(11) 3 . ?
Si1 O3 O1 128.82(11) 3 . ?
O2 O3 O1 100.93(8) 3 . ?
Si2 O3 O1 154.07(11) . 3_455 ?
Al1 O3 O1 36.45(8) 3 3_455 ?
Si1 O3 O1 36.45(8) 3 3_455 ?
O2 O3 O1 60.99(6) 3 3_455 ?
O1 O3 O1 161.87(9) . 3_455 ?
Si2 O3 O2 35.41(8) . 3_655 ?
Al1 O3 O2 149.56(10) 3 3_655 ?
Si1 O3 O2 149.56(10) 3 3_655 ?
O2 O3 O2 158.57(10) 3 3_655 ?
O1 O3 O2 59.43(6) . 3_655 ?
O1 O3 O2 138.61(8) 3_455 3_655 ?
Si2 O3 O5 34.62(7) . . ?
Al1 O3 O5 95.81(9) 3 . ?
Si1 O3 O5 95.81(9) 3 . ?
O2 O3 O5 103.19(7) 3 . ?
O1 O3 O5 60.72(6) . . ?
O1 O3 O5 121.73(7) 3_455 . ?
O2 O3 O5 60.99(5) 3_655 . ?
Si2 O3 O4 97.59(9) . 3 ?
Al1 O3 O4 34.71(7) 3 3 ?
Si1 O3 O4 34.71(7) 3 3 ?
O2 O3 O4 61.58(5) 3 3 ?
O1 O3 O4 113.64(7) . 3 ?
O1 O3 O4 60.66(5) 3_455 3 ?
O2 O3 O4 115.90(7) 3_655 3 ?
O5 O3 O4 62.97(5) . 3 ?
Si2 O3 K 112.00(9) . 3 ?
Al1 O3 K 108.28(11) 3 3 ?
Si1 O3 K 108.28(11) 3 3 ?
O2 O3 K 124.17(7) 3 3 ?
O1 O3 K 122.25(8) . 3 ?
O1 O3 K 72.03(7) 3_455 3 ?
O2 O3 K 76.59(6) 3_655 3 ?
O5 O3 K 127.35(6) . 3 ?
O4 O3 K 118.62(9) 3 3 ?
Si2 O3 O6 75.44(9) . 4 ?
Al1 O3 O6 82.34(9) 3 4 ?
Si1 O3 O6 82.34(9) 3 4 ?
O2 O3 O6 116.50(6) 3 4 ?
O1 O3 O6 111.61(6) . 4 ?
O1 O3 O6 80.19(6) 3_455 4 ?
O2 O3 O6 68.58(5) 3_655 4 ?
O5 O3 O6 56.42(5) . 4 ?
O4 O3 O6 55.74(5) 3 4 ?
K O3 O6 80.77(6) 3 4 ?
Si2 O5 Fe 123.38(11) . 7 ?
Si2 O5 Al 123.38(11) . 7 ?
Fe O5 Al 0.00(12) 7 7 ?
Si2 O5 Al 127.16(11) . . ?
Fe O5 Al 101.36(8) 7 . ?
Al O5 Al 101.36(8) 7 . ?
Si2 O5 M1 112.61(8) . 2_655 ?
Fe O5 M1 91.36(7) 7 2_655 ?
Al O5 M1 91.36(7) 7 2_655 ?
Al O5 M1 90.80(7) . 2_655 ?
Si2 O5 O5 155.63(11) . 7 ?
Fe O5 O5 51.02(7) 7 7 ?
Al O5 O5 51.02(7) 7 7 ?
Al O5 O5 50.33(7) . 7 ?
M1 O5 O5 91.70(7) 2_655 7 ?
Si2 O5 O1 34.73(8) . . ?
Fe O5 O1 150.57(9) 7 . ?
Al O5 O1 150.57(9) 7 . ?
Al O5 O1 92.74(8) . . ?
M1 O5 O1 114.35(6) 2_655 . ?
O5 O5 O1 136.20(9) 7 . ?
Si2 O5 O3 34.63(7) . . ?
Fe O5 O3 93.21(8) 7 . ?
Al O5 O3 93.21(8) 7 . ?
Al O5 O3 130.34(8) . . ?
M1 O5 O3 136.42(6) 2_655 . ?
O5 O5 O3 123.87(8) 7 . ?
O1 O5 O3 58.51(5) . . ?
Si2 O5 O2 33.68(7) . 3_655 ?
Fe O5 O2 116.77(8) 7 3_655 ?
Al O5 O2 116.77(8) 7 3_655 ?
Al O5 O2 140.91(9) . 3_655 ?
M1 O5 O2 80.50(5) 2_655 3_655 ?
O5 O5 O2 165.72(10) 7 3_655 ?
O1 O5 O2 58.03(5) . 3_655 ?
O3 O5 O2 58.94(5) . 3_655 ?
Si2 O5 O6 96.87(8) . 2 ?
Fe O5 O6 101.48(7) 7 2 ?
Al O5 O6 101.48(7) 7 2 ?
Al O5 O6 43.30(6) . 2 ?
M1 O5 O6 133.77(7) 2_655 2 ?
O5 O5 O6 65.11(6) 7 2 ?
O1 O5 O6 71.63(5) . 2 ?
O3 O5 O6 87.45(6) . 2 ?
O2 O5 O6 128.61(7) 3_655 2 ?
O2 Si1 O1 109.38(12) . 1_455 ?
O2 Si1 O4 112.67(12) . . ?
O1 Si1 O4 110.53(13) 1_455 . ?
O2 Si1 O3 106.50(13) . 3_445 ?
O1 Si1 O3 106.99(12) 1_455 3_445 ?
O4 Si1 O3 110.54(11) . 3_445 ?
O2 Si1 Al2 127.57(11) . 1_455 ?
O1 Si1 Al2 25.20(7) 1_455 1_455 ?
O4 Si1 Al2 86.20(9) . 1_455 ?
O3 Si1 Al2 111.53(10) 3_445 1_455 ?
O2 Si1 Si2 127.57(11) . 1_455 ?
O1 Si1 Si2 25.20(7) 1_455 1_455 ?
O4 Si1 Si2 86.20(9) . 1_455 ?
O3 Si1 Si2 111.53(10) 3_445 1_455 ?
Al2 Si1 Si2 0.00(7) 1_455 1_455 ?
O2 Si1 Al2 107.15(11) . 3_445 ?
O1 Si1 Al2 127.54(10) 1_455 3_445 ?
O4 Si1 Al2 87.86(8) . 3_445 ?
O3 Si1 Al2 25.24(7) 3_445 3_445 ?
Al2 Si1 Al2 122.63(7) 1_455 3_445 ?
Si2 Si1 Al2 122.63(7) 1_455 3_445 ?
O2 Si1 Si2 107.15(11) . 3_445 ?
O1 Si1 Si2 127.54(10) 1_455 3_445 ?
O4 Si1 Si2 87.86(8) . 3_445 ?
O3 Si1 Si2 25.24(7) 3_445 3_445 ?
Al2 Si1 Si2 122.63(7) 1_455 3_445 ?
Si2 Si1 Si2 122.63(7) 1_455 3_445 ?
Al2 Si1 Si2 0.00(10) 3_445 3_445 ?
O2 Si1 Al2 19.54(7) . 3_345 ?
O1 Si1 Al2 108.08(9) 1_455 3_345 ?
O4 Si1 Al2 96.13(9) . 3_345 ?
O3 Si1 Al2 123.96(11) 3_445 3_345 ?
Al2 Si1 Al2 118.82(7) 1_455 3_345 ?
Si2 Si1 Al2 118.82(7) 1_455 3_345 ?
Al2 Si1 Al2 118.55(8) 3_445 3_345 ?
Si2 Si1 Al2 118.55(8) 3_445 3_345 ?
O2 Si1 Si2 19.54(7) . 3_345 ?
O1 Si1 Si2 108.08(9) 1_455 3_345 ?
O4 Si1 Si2 96.13(9) . 3_345 ?
O3 Si1 Si2 123.96(11) 3_445 3_345 ?
Al2 Si1 Si2 118.82(7) 1_455 3_345 ?
Si2 Si1 Si2 118.82(7) 1_455 3_345 ?
Al2 Si1 Si2 118.55(8) 3_445 3_345 ?
Si2 Si1 Si2 118.55(8) 3_445 3_345 ?
Al2 Si1 Si2 0.00(9) 3_345 3_345 ?
O2 Si1 Fe 108.95(9) . 1_455 ?
O1 Si1 Fe 84.35(9) 1_455 1_455 ?
O4 Si1 Fe 30.79(7) . 1_455 ?
O3 Si1 Fe 136.35(10) 3_445 1_455 ?
Al2 Si1 Fe 63.43(6) 1_455 1_455 ?
Si2 Si1 Fe 63.43(6) 1_455 1_455 ?
Al2 Si1 Fe 117.22(7) 3_445 1_455 ?
Si2 Si1 Fe 117.22(7) 3_445 1_455 ?
Al2 Si1 Fe 89.42(6) 3_345 1_455 ?
Si2 Si1 Fe 89.42(6) 3_345 1_455 ?
O2 Si1 Al 108.95(9) . 1_455 ?
O1 Si1 Al 84.35(9) 1_455 1_455 ?
O4 Si1 Al 30.79(7) . 1_455 ?
O3 Si1 Al 136.35(10) 3_445 1_455 ?
Al2 Si1 Al 63.43(6) 1_455 1_455 ?
Si2 Si1 Al 63.43(6) 1_455 1_455 ?
Al2 Si1 Al 117.22(7) 3_445 1_455 ?
Si2 Si1 Al 117.22(7) 3_445 1_455 ?
Al2 Si1 Al 89.42(6) 3_345 1_455 ?
Si2 Si1 Al 89.42(6) 3_345 1_455 ?
Fe Si1 Al 0.00(8) 1_455 1_455 ?
Al2 O2 Si2 0.00(18) 3_345 3_345 ?
Al2 O2 Si1 140.92(13) 3_345 . ?
Si2 O2 Si1 140.92(13) 3_345 . ?
Al2 O2 O3 164.63(12) 3_345 3_445 ?
Si2 O2 O3 164.63(12) 3_345 3_445 ?
Si1 O2 O3 36.85(8) . 3_445 ?
Al2 O2 O1 36.73(8) 3_345 3_345 ?
Si2 O2 O1 36.73(8) 3_345 3_345 ?
Si1 O2 O1 164.68(12) . 3_345 ?
O3 O2 O1 138.96(8) 3_445 3_345 ?
Al2 O2 O3 35.53(8) 3_345 3_345 ?
Si2 O2 O3 35.53(8) 3_345 3_345 ?
Si1 O2 O3 128.98(11) . 3_345 ?
O3 O2 O3 158.57(10) 3_445 3_345 ?
O1 O2 O3 59.71(5) 3_345 3_345 ?
Al2 O2 O1 129.07(11) 3_345 1_455 ?
Si2 O2 O1 129.07(11) 3_345 1_455 ?
Si1 O2 O1 35.35(8) . 1_455 ?
O3 O2 O1 59.71(5) 3_445 1_455 ?
O1 O2 O1 158.63(9) 3_345 1_455 ?
O3 O2 O1 100.05(7) 3_345 1_455 ?
Al2 O2 O5 33.78(7) 3_345 3_345 ?
Si2 O2 O5 33.78(7) 3_345 3_345 ?
Si1 O2 O5 110.71(10) . 3_345 ?
O3 O2 O5 133.29(7) 3_445 3_345 ?
O1 O2 O5 60.49(5) 3_345 3_345 ?
O3 O2 O5 60.07(5) 3_345 3_345 ?
O1 O2 O5 117.60(7) 1_455 3_345 ?
Al2 O2 O4 110.77(10) 3_345 . ?
Si2 O2 O4 110.77(10) 3_345 . ?
Si1 O2 O4 33.73(8) . . ?
O3 O2 O4 60.52(5) 3_445 . ?
O1 O2 O4 133.31(7) 3_345 . ?
O3 O2 O4 117.66(7) 3_345 . ?
O1 O2 O4 59.90(5) 1_455 . ?
O5 O2 O4 77.95(6) 3_345 . ?
Al2 O2 K 108.42(11) 3_345 3_445 ?
Si2 O2 K 108.42(11) 3_345 3_445 ?
Si1 O2 K 108.35(9) . 3_445 ?
O3 O2 K 71.60(6) 3_445 3_445 ?
O1 O2 K 71.79(7) 3_345 3_445 ?
O3 O2 K 117.03(6) 3_345 3_445 ?
O1 O2 K 116.95(8) 1_455 3_445 ?
O5 O2 K 124.80(9) 3_345 3_445 ?
O4 O2 K 124.70(6) . 3_445 ?
Al2 O2 M1 76.15(8) 3_345 4_445 ?
Si2 O2 M1 76.15(8) 3_345 4_445 ?
Si1 O2 M1 76.15(8) . 4_445 ?
O3 O2 M1 89.97(5) 3_445 4_445 ?
O1 O2 M1 89.96(5) 3_345 4_445 ?
O3 O2 M1 102.01(5) 3_345 4_445 ?
O1 O2 M1 101.88(6) 1_455 4_445 ?
O5 O2 M1 43.40(3) 3_345 4_445 ?
O4 O2 M1 43.44(4) . 4_445 ?
K O2 M1 116.26(7) 3_445 4_445 ?
Si1 O4 Fe 123.45(11) . 1_455 ?
Si1 O4 Al 123.45(11) . 1_455 ?
Fe O4 Al 0.00(14) 1_455 1_455 ?
Si1 O4 Fe 127.24(10) . 5 ?
Fe O4 Fe 101.28(9) 1_455 5 ?
Al O4 Fe 101.28(9) 1_455 5 ?
Si1 O4 Al 127.24(10) . 5 ?
Fe O4 Al 101.28(9) 1_455 5 ?
Al O4 Al 101.28(9) 1_455 5 ?
Fe O4 Al 0.00(13) 5 5 ?
Si1 O4 M1 112.41(9) . 4_445 ?
Fe O4 M1 91.46(7) 1_455 4_445 ?
Al O4 M1 91.46(7) 1_455 4_445 ?
Fe O4 M1 90.80(7) 5 4_445 ?
Al O4 M1 90.80(7) 5 4_445 ?
Si1 O4 O4 155.75(13) . 5_455 ?
Fe O4 O4 50.96(7) 1_455 5_455 ?
Al O4 O4 50.96(7) 1_455 5_455 ?
Fe O4 O4 50.31(7) 5 5_455 ?
Al O4 O4 50.31(7) 5 5_455 ?
M1 O4 O4 91.78(7) 4_445 5_455 ?
Si1 O4 O1 34.70(8) . 1_455 ?
Fe O4 O1 93.26(8) 1_455 1_455 ?
Al O4 O1 93.26(8) 1_455 1_455 ?
Fe O4 O1 130.35(8) 5 1_455 ?
Al O4 O1 130.35(8) 5 1_455 ?
M1 O4 O1 136.38(6) 4_445 1_455 ?
O4 O4 O1 123.88(9) 5_455 1_455 ?
Si1 O4 O3 34.75(7) . 3_445 ?
Fe O4 O3 150.67(9) 1_455 3_445 ?
Al O4 O3 150.67(9) 1_455 3_445 ?
Fe O4 O3 92.80(7) 5 3_445 ?
Al O4 O3 92.80(7) 5 3_445 ?
M1 O4 O3 114.14(7) 4_445 3_445 ?
O4 O4 O3 136.29(8) 5_455 3_445 ?
O1 O4 O3 58.55(5) 1_455 3_445 ?
Si1 O4 O2 33.60(7) . . ?
Fe O4 O2 116.93(8) 1_455 . ?
Al O4 O2 116.93(8) 1_455 . ?
Fe O4 O2 140.81(9) 5 . ?
Al O4 O2 140.81(9) 5 . ?
M1 O4 O2 80.36(5) 4_445 . ?
O4 O4 O2 165.77(8) 5_455 . ?
O1 O4 O2 59.03(6) 1_455 . ?
O3 O4 O2 57.91(5) 3_445 . ?
Si1 O4 O6 97.03(8) . 2 ?
Fe O4 O6 101.35(8) 1_455 2 ?
Al O4 O6 101.35(8) 1_455 2 ?
Fe O4 O6 43.30(6) 5 2 ?
Al O4 O6 43.30(6) 5 2 ?
M1 O4 O6 133.77(6) 4_445 2 ?
O4 O4 O6 65.04(6) 5_455 2 ?
O1 O4 O6 87.46(6) 1_455 2 ?
O3 O4 O6 71.80(5) 3_445 2 ?
O2 O4 O6 128.66(6) . 2 ?
Fe O6 Al 0.00(9) 2 2 ?
Fe O6 Fe 102.14(9) 2 6_556 ?
Al O6 Fe 102.14(9) 2 6_556 ?
Fe O6 Al 102.14(9) 2 6_556 ?
Al O6 Al 102.14(9) 2 6_556 ?
Fe O6 Al 0.00(12) 6_556 6_556 ?
Fe O6 M1 93.45(8) 2 . ?
Al O6 M1 93.45(8) 2 . ?
Fe O6 M1 93.59(7) 6_556 . ?
Al O6 M1 93.59(7) 6_556 . ?
Fe O6 O6 51.07(7) 2 5_556 ?
Al O6 O6 51.07(7) 2 5_556 ?
Fe O6 O6 51.07(7) 6_556 5_556 ?
Al O6 O6 51.07(7) 6_556 5_556 ?
M1 O6 O6 95.61(8) . 5_556 ?
Fe O6 O4 145.37(9) 2 2 ?
Al O6 O4 145.37(9) 2 2 ?
Fe O6 O4 43.83(6) 6_556 2 ?
Al O6 O4 43.83(6) 6_556 2 ?
M1 O6 O4 84.41(5) . 2 ?
O6 O6 O4 94.63(8) 5_556 2 ?
Fe O6 O5 43.91(6) 2 2 ?
Al O6 O5 43.91(6) 2 2 ?
Fe O6 O5 145.47(9) 6_556 2 ?
Al O6 O5 145.47(9) 6_556 2 ?
M1 O6 O5 84.30(5) . 2 ?
O6 O6 O5 94.72(8) 5_556 2 ?
O4 O6 O5 165.98(7) 2 2 ?
Fe O6 O4 42.78(6) 2 2_455 ?
Al O6 O4 42.78(6) 2 2_455 ?
Fe O6 O4 101.77(8) 6_556 2_455 ?
Al O6 O4 101.77(8) 6_556 2_455 ?
M1 O6 O4 135.59(7) . 2_455 ?
O6 O6 O4 65.05(6) 5_556 2_455 ?
O4 O6 O4 133.97(8) 2 2_455 ?
O5 O6 O4 59.83(5) 2 2_455 ?
Fe O6 O5 101.80(8) 2 4_545 ?
Al O6 O5 101.80(8) 2 4_545 ?
Fe O6 O5 42.69(6) 6_556 4_545 ?
Al O6 O5 42.69(6) 6_556 4_545 ?
M1 O6 O5 135.65(6) . 4_545 ?
O6 O6 O5 65.03(7) 5_556 4_545 ?
O4 O6 O5 59.77(5) 2 4_545 ?
O5 O6 O5 134.04(7) 2 4_545 ?
O4 O6 O5 74.22(5) 2_455 4_545 ?
Fe O6 O4 101.26(8) 2 6_656 ?
Al O6 O4 101.26(8) 2 6_656 ?
Fe O6 O4 42.45(6) 6_556 6_656 ?
Al O6 O4 42.45(6) 6_556 6_656 ?
M1 O6 O4 51.14(4) . 6_656 ?
O6 O6 O4 64.42(6) 5_556 6_656 ?
O4 O6 O4 51.54(5) 2 6_656 ?
O5 O6 O4 124.75(6) 2 6_656 ?
O4 O6 O4 129.48(6) 2_455 6_656 ?
O5 O6 O4 84.90(5) 4_545 6_656 ?
Fe O6 O5 42.44(6) 2 8_456 ?
Al O6 O5 42.44(6) 2 8_456 ?
Fe O6 O5 101.39(8) 6_556 8_456 ?
Al O6 O5 101.39(8) 6_556 8_456 ?
M1 O6 O5 51.02(4) . 8_456 ?
O6 O6 O5 64.53(7) 5_556 8_456 ?
O4 O6 O5 124.75(6) 2 8_456 ?
O5 O6 O5 51.52(5) 2 8_456 ?
O4 O6 O5 84.96(5) 2_455 8_456 ?
O5 O6 O5 129.56(6) 4_545 8_456 ?
O4 O6 O5 73.82(5) 6_656 8_456 ?
O6 M1 O6 180.000(1) . 7_556 ?
O6 M1 O5 79.98(5) . 8_456 ?
O6 M1 O5 100.02(5) 7_556 8_456 ?
O6 M1 O5 100.02(5) . 2_655 ?
O6 M1 O5 79.98(5) 7_556 2_655 ?
O5 M1 O5 180.0 8_456 2_655 ?
O6 M1 O4 79.82(5) . 6_656 ?
O6 M1 O4 100.18(5) 7_556 6_656 ?
O5 M1 O4 98.92(5) 8_456 6_656 ?
O5 M1 O4 81.08(5) 2_655 6_656 ?
O6 M1 O4 100.18(5) . 4_455 ?
O6 M1 O4 79.82(5) 7_556 4_455 ?
O5 M1 O4 81.08(5) 8_456 4_455 ?
O5 M1 O4 98.92(5) 2_655 4_455 ?
O4 M1 O4 180.0 6_656 4_455 ?
O6 M1 Al 90.07(5) . 8_456 ?
O6 M1 Al 89.93(5) 7_556 8_456 ?
O5 M1 Al 40.58(5) 8_456 8_456 ?
O5 M1 Al 139.42(5) 2_655 8_456 ?
O4 M1 Al 139.50(5) 6_656 8_456 ?
O4 M1 Al 40.50(4) 4_455 8_456 ?
O6 M1 Al 89.93(5) . 2_655 ?
O6 M1 Al 90.07(5) 7_556 2_655 ?
O5 M1 Al 139.42(5) 8_456 2_655 ?
O5 M1 Al 40.58(5) 2_655 2_655 ?
O4 M1 Al 40.50(4) 6_656 2_655 ?
O4 M1 Al 139.50(5) 4_455 2_655 ?
Al M1 Al 180.00(6) 8_456 2_655 ?
O6 M1 Fe 90.07(5) . 8_456 ?
O6 M1 Fe 89.93(5) 7_556 8_456 ?
O5 M1 Fe 40.58(5) 8_456 8_456 ?
O5 M1 Fe 139.42(5) 2_655 8_456 ?
O4 M1 Fe 139.50(5) 6_656 8_456 ?
O4 M1 Fe 40.50(4) 4_455 8_456 ?
Al M1 Fe 0.00(7) 8_456 8_456 ?
Al M1 Fe 180.0 2_655 8_456 ?
O6 M1 Fe 89.93(5) . 2_655 ?
O6 M1 Fe 90.07(5) 7_556 2_655 ?
O5 M1 Fe 139.42(5) 8_456 2_655 ?
O5 M1 Fe 40.58(5) 2_655 2_655 ?
O4 M1 Fe 40.50(4) 6_656 2_655 ?
O4 M1 Fe 139.50(5) 4_455 2_655 ?
Al M1 Fe 180.00(6) 8_456 2_655 ?
Al M1 Fe 0.00(8) 2_655 2_655 ?
Fe M1 Fe 180.00(6) 8_456 2_655 ?
O6 M1 Al 39.92(5) . 2 ?
O6 M1 Al 140.08(5) 7_556 2 ?
O5 M1 Al 40.06(5) 8_456 2 ?
O5 M1 Al 139.94(5) 2_655 2 ?
O4 M1 Al 89.57(4) 6_656 2 ?
O4 M1 Al 90.43(4) 4_455 2 ?
Al M1 Al 60.09(6) 8_456 2 ?
Al M1 Al 119.91(6) 2_655 2 ?
Fe M1 Al 60.09(6) 8_456 2 ?
Fe M1 Al 119.91(6) 2_655 2 ?
O6 M1 Al 140.08(5) . 8_556 ?
O6 M1 Al 39.92(5) 7_556 8_556 ?
O5 M1 Al 139.94(5) 8_456 8_556 ?
O5 M1 Al 40.06(5) 2_655 8_556 ?
O4 M1 Al 90.43(4) 6_656 8_556 ?
O4 M1 Al 89.57(4) 4_455 8_556 ?
Al M1 Al 119.91(6) 8_456 8_556 ?
Al M1 Al 60.09(6) 2_655 8_556 ?
Fe M1 Al 119.91(6) 8_456 8_556 ?
Fe M1 Al 60.09(6) 2_655 8_556 ?
Al M1 Al 180.0 2 8_556 ?
 
_diffrn_measured_fraction_theta_max    0.990
_diffrn_reflns_theta_full              44.98
_diffrn_measured_fraction_theta_full   0.990
_refine_diff_density_max    1.104
_refine_diff_density_min   -1.060
_refine_diff_density_rms    0.244
